Loading in 2 Seconds...
Loading in 2 Seconds...
Electronic Structure of Rocksalt Copper Monoxide: A Proxy for High Temperature Superconductivity. Paul M. Grant IBM Research Staff Member, Emeritus www.w2agz.com [email protected] Journal of Physics: Conference Series 129 (2008) 012042
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Paul M. GrantIBM Research Staff Member, Emerituswww.w2agz.com
Journal of Physics: Conference Series 129 (2008) 012042
Abstract. Cubic rocksalt copper monoxide, in contrast to its lighter transition metal neighbours, does not exist in nature nor has it yet been successfully synthesized. Nonetheless, its numerical study as a structurally simpler proxy for the layered cuprate perovskites may prove useful in probing the source of high temperature superconductivity in the latter family of compounds. We report plane-wave pseudopotential DFT (LDA+U) results for both cubic and tetragonal CuO and find rather surprisingly a metallic band structure persists for 0 < U < 6 eV, and c/a = 1 with a Mott-Hubbard gap opening only for finite U under a tetragonal distortion, e.g., above c/a = 1.1 for U = 6. The metallic states display a Fermi surface with clear nesting tendencies suggesting that high temperature superconductivity in copper oxide compounds may be at least initially mediated by Jahn-Teller electron-phonon coupling as originally proposed by Bednorz and Mueller.
“Should be Metals, But Aren’t” (Charge Transfer Insulators, Instead)
After Imada, et al, RMP 70, 1039 (1998)
TMO 3d Config Properties
MnO 5 MH-CTI (5.6)
FeO 6 MH-CTI (5.9)
CoO 7 MH-CTI (6.3)
NiO 8 MH-CTI (6.5)
XX Doesn\'t Exist!
See Imada, Fujimore, Tokura, RPM 70 (1988)
Tenorite (Monoclinic CuO)
QUANTUM-ESPRESSO Suit of Codes
DFT (LDA+U) plus electron-phonon
Graphics by Tone Kolalj (XCrysDen)
G2 = 40 Ry ρ = 320 Ry
Convergence ≤ 10-6 Ry
“Smearing” = Methfessel-Paxton
Psuedopotentials: Ultrasoft, XC = Perdew-ZungerCu: 3d94s2 O: 2s22p4
c/a = 1.36
U = 6
U = 0
1.0 1.1 1.115 1.2 1.36
U = 0 d-spin-pdos Cu1
U = 5 d-spin-pdos Cu1
W. Siemons (PhD Thesis, Stanford)
λ ~ 0.6 – 0.7
k << EF
σ = 0.04
c-rs-CuO is metallic and thus a proxy for HTSC cuprates.
e-p λ ~ 0.6 – 0.7 consistent with TC ~ 20 – 50 K.
t-rs-CuO becomes a MH-CTI for c/a >~ 1.1, U > 3 eV.
c/a < 1.1, t-rs-CuO is “self-doped” metal.
DFT (LDA+U) + proxy structures a useful exploratory tool for nano-material discovery.
Compute e-p coupling λ as f(c/a,U) for t-rs-CuO.
Compute TN, µ*, BCS prefactor, then TC .
Compute isotope shift.
Calculate optical & transport properties as f(c/a).
Investigate larger values of a-lattice constant